#------------------------------------------------------------------------------
#$Date: 2017-03-05 08:29:33 +0200 (Sun, 05 Mar 2017) $
#$Revision: 193925 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/24/20/2242050.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2242050
loop_
_publ_author_name
'Ben Smail, Ridha'
'Zid, Mohamed Faouzi'
_publ_section_title
;
 K₁₊₂ₓNi~1{-~x}Fe₂(AsO₄)₃ (x = 0,125): un
 nouvel arséniate à structure de type α-CrPO₄
;
_journal_coeditor_code           VN2121
_journal_issue                   2
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              239
_journal_page_last               245
_journal_paper_doi               10.1107/S2056989017000950
_journal_volume                  73
_journal_year                    2017
_chemical_formula_iupac          'K1.25 Ni0.88 Fe2 (As O4)3'
_chemical_formula_sum            'As3 Fe2 K1.25 Ni0.88 O12'
_chemical_formula_weight         628.71
_chemical_name_systematic
;
Potassium nickel diiron(III) tris[arsenate(V)]
;
_space_group_crystal_system      orthorhombic
_space_group_IT_number           74
_space_group_name_Hall           '-I 2c 2c'
_space_group_name_H-M_alt        'I b m m'
_symmetry_space_group_name_Hall  '-I 2c 2c'
_symmetry_space_group_name_H-M   'I b m m'
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.737(2)
_cell_length_b                   10.773(3)
_cell_length_c                   13.574(3)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      14.48
_cell_measurement_theta_min      10.83
_cell_volume                     985.2(5)
_computing_cell_refinement
;
CAD-4 EXPRESS (Duisenberg, 1992; Macíček & Yordanov, 1992)
;
_computing_data_collection
;
CAD-4 EXPRESS (Duisenberg, 1992; Macíček & Yordanov, 1992)
;
_computing_data_reduction
;
XCAD4 (Harms & Wocadlo, 1995)
;
_computing_molecular_graphics
;
DIAMOND (Brandenburg, 2006)
;
_computing_publication_material
;
WinGX (Farrugia, 2012) & publCIF (Westrip, 2010)
;
_computing_structure_refinement
;
SHELXL2014 (Sheldrick, 2015)
;
_computing_structure_solution
;
SHELXS97 (Sheldrick, 2008)
;
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Enraf--Nonius CAD-4'
_diffrn_measurement_method       ω/2θ
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0256
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -1
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            1323
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.953
_diffrn_reflns_theta_min         3.001
_diffrn_standards_decay_%        1
_diffrn_standards_interval_count 120
_diffrn_standards_number         2
_exptl_absorpt_coefficient_mu    15.161
_exptl_absorpt_correction_T_max  0.9992
_exptl_absorpt_correction_T_min  0.3724
_exptl_absorpt_correction_type   psi-scan
_exptl_absorpt_process_details
;
(North et al., 1968)
;
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    4.239
_exptl_crystal_description       prism
_exptl_crystal_F_000             1181
_exptl_crystal_size_max          0.252
_exptl_crystal_size_mid          0.182
_exptl_crystal_size_min          0.072
_refine_diff_density_max         1.122
_refine_diff_density_min         -0.920
_refine_ls_extinction_coef       0.0016(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method
;
SHELXL2014 (Sheldrick, 2015)
;
_refine_ls_goodness_of_fit_ref   1.102
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     58
_refine_ls_number_reflns         591
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.102
_refine_ls_R_factor_all          0.0308
_refine_ls_R_factor_gt           0.0284
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0629P)²+3.0716P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0872
_refine_ls_wR_factor_ref         0.0888
_reflns_number_gt                548
_reflns_number_total             591
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            vn2121sup1.cif
_cod_data_source_block           I
_cod_database_code               2242050
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.051
_shelx_estimated_absorpt_t_max   0.336
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z+1/2'
'x, -y, -z+1/2'
'-x, y, -z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1'
'x+1/2, -y+1/2, -z+1'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z-1/2'
'-x, y, z-1/2'
'x, -y, z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z'
'-x+1/2, y+1/2, z'
'x+1/2, -y+1/2, z+1/2'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_occupancy
Fe Fe 0.2500 0.2500 0.63616(6) 0.0043(3) Uani d 1
Ni Ni 0.0000 0.5000 0.5000 0.0067(3) Uani d 0.875
K K1 0.0797(3) 0.0000 0.2500 0.0219(6) Uani d 1
K K2 0.5000 0.5000 0.5000 0.027(2) Uani d 0.25
As As1 0.2500 0.2500 0.42905(4) 0.0068(3) Uani d 1
As As2 0.07167(11) 0.5000 0.7500 0.0059(3) Uani d 1
O O1 0.2062(5) 0.3657(3) 0.5158(2) 0.0094(6) Uani d 1
O O2 -0.0672(6) 0.5000 0.6470(3) 0.0105(9) Uani d 1
O O3 0.0501(5) 0.2095(3) 0.3635(2) 0.0152(7) Uani d 1
O O4 0.2254(6) 0.3742(4) 0.7500 0.0093(9) Uani d 1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
1 6 5
3 -4 5
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O4 Fe O4 . 13_556 82.21(17)
O4 Fe O3 . 4_556 93.27(16)
O4 Fe O3 13_556 4_556 86.55(15)
O4 Fe O3 . 7 86.55(15)
O4 Fe O3 13_556 7 93.27(16)
O3 Fe O3 4_556 7 179.77(19)
O4 Fe O1 . . 100.94(12)
O4 Fe O1 13_556 . 175.01(13)
O3 Fe O1 4_556 . 89.40(13)
O3 Fe O1 7 . 90.79(14)
O4 Fe O1 . 6_554 175.02(14)
O4 Fe O1 13_556 6_554 100.94(12)
O3 Fe O1 4_556 6_554 90.79(14)
O3 Fe O1 7 6_554 89.40(13)
O1 Fe O1 . 6_554 76.19(17)
O4 Fe As1 . . 138.90(9)
O4 Fe As1 13_556 . 138.90(9)
O3 Fe As1 4_556 . 90.12(9)
O3 Fe As1 7 . 90.12(9)
O1 Fe As1 . . 38.10(8)
O1 Fe As1 6_554 . 38.09(8)
O4 Fe K2 . 6_554 145.08(12)
O4 Fe K2 13_556 6_554 86.44(10)
O3 Fe K2 4_556 6_554 53.01(10)
O3 Fe K2 7 6_554 127.13(9)
O1 Fe K2 . 6_554 88.80(9)
O1 Fe K2 6_554 6_554 39.59(9)
As1 Fe K2 . 6_554 59.807(14)
O4 Fe K2 . . 86.44(10)
O4 Fe K2 13_556 . 145.08(12)
O3 Fe K2 4_556 . 127.13(9)
O3 Fe K2 7 . 53.01(10)
O1 Fe K2 . . 39.59(9)
O1 Fe K2 6_554 . 88.80(9)
As1 Fe K2 . . 59.807(14)
K2 Fe K2 6_554 . 119.61(3)
O4 Fe K1 . 5 44.10(12)
O4 Fe K1 13_556 5 96.21(11)
O3 Fe K1 4_556 5 135.79(11)
O3 Fe K1 7 5 44.07(9)
O1 Fe K1 . 5 88.72(9)
O1 Fe K1 6_554 5 131.25(10)
As1 Fe K1 . 5 113.876(15)
K2 Fe K1 6_554 5 170.81(3)
K2 Fe K1 . 5 54.545(14)
O4 Fe K1 . 9_556 96.21(11)
O4 Fe K1 13_556 9_556 44.10(12)
O3 Fe K1 4_556 9_556 44.07(9)
O3 Fe K1 7 9_556 135.79(11)
O1 Fe K1 . 9_556 131.25(10)
O1 Fe K1 6_554 9_556 88.72(9)
As1 Fe K1 . 9_556 113.876(15)
K2 Fe K1 6_554 9_556 54.545(15)
K2 Fe K1 . 9_556 170.81(3)
K1 Fe K1 5 9_556 132.25(3)
O1 Ni O1 . 12_565 91.64(18)
O1 Ni O1 . 4_556 88.36(18)
O1 Ni O1 12_565 4_556 180.0
O1 Ni O1 . 9_566 180.0
O1 Ni O1 12_565 9_566 88.36(18)
O1 Ni O1 4_556 9_566 91.64(18)
O1 Ni O2 . . 92.81(13)
O1 Ni O2 12_565 . 92.81(13)
O1 Ni O2 4_556 . 87.19(13)
O1 Ni O2 9_566 . 87.19(13)
O1 Ni O2 . 9_566 87.19(13)
O1 Ni O2 12_565 9_566 87.19(13)
O1 Ni O2 4_556 9_566 92.81(13)
O1 Ni O2 9_566 9_566 92.81(13)
O2 Ni O2 . 9_566 180.0
O1 Ni K2 . 1_455 133.53(9)
O1 Ni K2 12_565 1_455 133.53(9)
O1 Ni K2 4_556 1_455 46.47(9)
O1 Ni K2 9_566 1_455 46.47(9)
O2 Ni K2 . 1_455 77.21(12)
O2 Ni K2 9_566 1_455 102.79(12)
O1 Ni K2 . . 46.47(9)
O1 Ni K2 12_565 . 46.47(9)
O1 Ni K2 4_556 . 133.53(9)
O1 Ni K2 9_566 . 133.53(9)
O2 Ni K2 . . 102.79(12)
O2 Ni K2 9_566 . 77.21(12)
K2 Ni K2 1_455 . 180.0
O3 K1 O3 . 3 171.66(16)
O3 K1 O3 . 12 110.90(15)
O3 K1 O3 3 12 68.45(15)
O3 K1 O3 . 10_556 68.45(15)
O3 K1 O3 3 10_556 110.90(15)
O3 K1 O3 12 10_556 171.66(16)
O3 K1 O4 . 5_444 110.09(12)
O3 K1 O4 3 5_444 61.98(9)
O3 K1 O4 12 5_444 61.98(9)
O3 K1 O4 10_556 5_444 110.09(12)
O3 K1 O4 . 7_455 61.98(9)
O3 K1 O4 3 7_455 110.09(12)
O3 K1 O4 12 7_455 110.09(12)
O3 K1 O4 10_556 7_455 61.98(9)
O4 K1 O4 5_444 7_455 59.17(17)
O3 K1 O2 . 14_546 77.16(9)
O3 K1 O2 3 14_546 110.34(10)
O3 K1 O2 12 14_546 77.16(9)
O3 K1 O2 10_556 14_546 110.34(10)
O4 K1 O2 5_444 14_546 138.57(8)
O4 K1 O2 7_455 14_546 138.57(8)
O3 K1 O2 . 5_544 110.34(10)
O3 K1 O2 3 5_544 77.16(9)
O3 K1 O2 12 5_544 110.34(10)
O3 K1 O2 10_556 5_544 77.16(9)
O4 K1 O2 5_444 5_544 138.57(8)
O4 K1 O2 7_455 5_544 138.57(8)
O2 K1 O2 14_546 5_544 60.88(19)
O3 K1 As2 . 5_544 94.17(8)
O3 K1 As2 3 5_544 94.17(8)
O3 K1 As2 12 5_544 94.17(8)
O3 K1 As2 10_556 5_544 94.17(8)
O4 K1 As2 5_444 5_544 150.41(9)
O4 K1 As2 7_455 5_544 150.41(9)
O2 K1 As2 14_546 5_544 30.44(9)
O2 K1 As2 5_544 5_544 30.44(9)
O3 K1 As2 . 5_444 85.83(8)
O3 K1 As2 3 5_444 85.83(8)
O3 K1 As2 12 5_444 85.83(8)
O3 K1 As2 10_556 5_444 85.83(8)
O4 K1 As2 5_444 5_444 29.59(9)
O4 K1 As2 7_455 5_444 29.59(9)
O2 K1 As2 14_546 5_444 149.56(9)
O2 K1 As2 5_544 5_444 149.56(9)
As2 K1 As2 5_544 5_444 180.0
O3 K1 K2 . 5_444 122.97(7)
O3 K1 K2 3 5_444 55.47(7)
O3 K1 K2 12 5_444 122.97(7)
O3 K1 K2 10_556 5_444 55.47(7)
O4 K1 K2 5_444 5_444 82.19(3)
O4 K1 K2 7_455 5_444 82.19(3)
O2 K1 K2 14_546 5_444 129.43(10)
O2 K1 K2 5_544 5_444 68.55(9)
As2 K1 K2 5_544 5_444 98.99(3)
As2 K1 K2 5_444 5_444 81.01(3)
O3 K1 K2 . 6_554 55.46(7)
O3 K1 K2 3 6_554 122.97(7)
O3 K1 K2 12 6_554 55.47(7)
O3 K1 K2 10_556 6_554 122.97(7)
O4 K1 K2 5_444 6_554 82.19(3)
O4 K1 K2 7_455 6_554 82.19(3)
O2 K1 K2 14_546 6_554 68.55(9)
O2 K1 K2 5_544 6_554 129.43(10)
As2 K1 K2 5_544 6_554 98.99(3)
As2 K1 K2 5_444 6_554 81.01(3)
K2 K1 K2 5_444 6_554 162.02(6)
O1 K2 O1 9_666 12_565 108.00(14)
O1 K2 O1 9_666 4_656 72.00(14)
O1 K2 O1 12_565 4_656 180.0
O1 K2 O1 9_666 . 180.0
O1 K2 O1 12_565 . 72.00(14)
O1 K2 O1 4_656 . 108.00(14)
O1 K2 O3 9_666 14_556 60.73(10)
O1 K2 O3 12_565 14_556 65.57(10)
O1 K2 O3 4_656 14_556 114.43(10)
O1 K2 O3 . 14_556 119.27(10)
O1 K2 O3 9_666 6_554 119.27(10)
O1 K2 O3 12_565 6_554 114.43(10)
O1 K2 O3 4_656 6_554 65.57(10)
O1 K2 O3 . 6_554 60.73(10)
O3 K2 O3 14_556 6_554 180.0
O1 K2 O3 9_666 15 65.57(10)
O1 K2 O3 12_565 15 60.73(10)
O1 K2 O3 4_656 15 119.27(10)
O1 K2 O3 . 15 114.43(10)
O3 K2 O3 14_556 15 79.69(13)
O3 K2 O3 6_554 15 100.31(13)
O1 K2 O3 9_666 7 114.43(10)
O1 K2 O3 12_565 7 119.27(10)
O1 K2 O3 4_656 7 60.73(10)
O1 K2 O3 . 7 65.57(10)
O3 K2 O3 14_556 7 100.31(13)
O3 K2 O3 6_554 7 79.69(13)
O3 K2 O3 15 7 180.0
O1 K2 As1 9_666 9_666 30.70(7)
O1 K2 As1 12_565 9_666 84.61(7)
O1 K2 As1 4_656 9_666 95.39(7)
O1 K2 As1 . 9_666 149.30(7)
O3 K2 As1 14_556 9_666 30.21(6)
O3 K2 As1 6_554 9_666 149.79(6)
O3 K2 As1 15 9_666 67.56(7)
O3 K2 As1 7 9_666 112.44(7)
O1 K2 As1 9_666 15 84.61(7)
O1 K2 As1 12_565 15 30.70(7)
O1 K2 As1 4_656 15 149.30(7)
O1 K2 As1 . 15 95.39(7)
O3 K2 As1 14_556 15 67.56(7)
O3 K2 As1 6_554 15 112.44(7)
O3 K2 As1 15 15 30.21(6)
O3 K2 As1 7 15 149.79(6)
As1 K2 As1 9_666 15 71.54(2)
O1 K2 As1 9_666 7 95.39(7)
O1 K2 As1 12_565 7 149.30(7)
O1 K2 As1 4_656 7 30.70(7)
O1 K2 As1 . 7 84.61(7)
O3 K2 As1 14_556 7 112.44(7)
O3 K2 As1 6_554 7 67.56(7)
O3 K2 As1 15 7 149.79(6)
O3 K2 As1 7 7 30.21(6)
As1 K2 As1 9_666 7 108.46(2)
As1 K2 As1 15 7 180.00(2)
O1 K2 As1 9_666 . 149.30(7)
O1 K2 As1 12_565 . 95.39(7)
O1 K2 As1 4_656 . 84.61(7)
O1 K2 As1 . . 30.70(7)
O3 K2 As1 14_556 . 149.79(6)
O3 K2 As1 6_554 . 30.21(6)
O3 K2 As1 15 . 112.44(7)
O3 K2 As1 7 . 67.56(7)
As1 K2 As1 9_666 . 180.0
As1 K2 As1 15 . 108.46(2)
As1 K2 As1 7 . 71.54(2)
O3 As1 O3 6_554 . 115.7(2)
O3 As1 O1 6_554 6_554 114.24(16)
O3 As1 O1 . 6_554 108.02(17)
O3 As1 O1 6_554 . 108.02(17)
O3 As1 O1 . . 114.24(16)
O1 As1 O1 6_554 . 94.9(2)
O3 As1 Fe 6_554 . 122.14(12)
O3 As1 Fe . . 122.14(12)
O1 As1 Fe 6_554 . 47.43(10)
O1 As1 Fe . . 47.43(10)
O3 As1 K2 6_554 . 62.21(12)
O3 As1 K2 . . 140.81(12)
O1 As1 K2 6_554 . 107.41(11)
O1 As1 K2 . . 46.24(11)
Fe As1 K2 . . 73.134(11)
O3 As1 K2 6_554 6_554 140.80(12)
O3 As1 K2 . 6_554 62.21(12)
O1 As1 K2 6_554 6_554 46.23(11)
O1 As1 K2 . 6_554 107.41(11)
Fe As1 K2 . 6_554 73.134(11)
K2 As1 K2 . 6_554 146.27(2)
O3 As1 K1 6_554 . 95.04(13)
O3 As1 K1 . . 39.86(12)
O1 As1 K1 6_554 . 88.62(11)
O1 As1 K1 . . 152.66(11)
Fe As1 K1 . . 129.701(14)
K2 As1 K1 . . 155.88(2)
K2 As1 K1 6_554 . 57.180(19)
O3 As1 K1 6_554 13 39.86(12)
O3 As1 K1 . 13 95.04(13)
O1 As1 K1 6_554 13 152.66(11)
O1 As1 K1 . 13 88.62(11)
Fe As1 K1 . 13 129.701(14)
K2 As1 K1 . 13 57.180(18)
K2 As1 K1 6_554 13 155.88(2)
K1 As1 K1 . 13 100.60(3)
O2 As2 O2 10_557 . 112.4(3)
O2 As2 O4 10_557 . 109.74(11)
O2 As2 O4 . . 109.74(11)
O2 As2 O4 10_557 3_566 109.74(11)
O2 As2 O4 . 3_566 109.74(11)
O4 As2 O4 . 3_566 105.2(3)
O2 As2 K1 10_557 5_455 56.20(15)
O2 As2 K1 . 5_455 56.20(15)
O4 As2 K1 . 5_455 127.38(15)
O4 As2 K1 3_566 5_455 127.38(15)
O2 As2 K1 10_557 5 123.80(15)
O2 As2 K1 . 5 123.80(15)
O4 As2 K1 . 5 52.62(15)
O4 As2 K1 3_566 5 52.62(15)
K1 As2 K1 5_455 5 180.0
As1 O1 Ni . . 123.99(17)
As1 O1 Fe . . 94.47(13)
Ni O1 Fe . . 127.73(17)
As1 O1 K2 . . 103.06(15)
Ni O1 K2 . . 97.08(12)
Fe O1 K2 . . 107.88(13)
As2 O2 Ni . . 133.4(2)
As2 O2 K1 . 5_455 93.36(19)
Ni O2 K1 . 5_455 133.23(19)
As1 O3 Fe . 7_455 136.97(19)
As1 O3 K1 . . 117.12(17)
Fe O3 K1 7_455 . 104.24(13)
As1 O3 K2 . 6_554 87.58(13)
Fe O3 K2 7_455 6_554 92.78(12)
K1 O3 K2 . 6_554 74.37(9)
As2 O4 Fe . . 124.58(13)
As2 O4 Fe . 13_556 124.58(13)
Fe O4 Fe . 13_556 97.79(17)
As2 O4 K1 . 5 97.79(18)
Fe O4 K1 . 5 104.58(14)
Fe O4 K1 13_556 5 104.58(14)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Fe O4 . 2.051(3) y
Fe O4 13_556 2.051(3) y
Fe O3 4_556 2.069(3) y
Fe O3 7 2.069(3) y
Fe O1 . 2.077(3) y
Fe O1 6_554 2.077(3) y
Fe As1 . 2.8113(12) ?
Fe K2 6_554 3.6751(8) ?
Fe K2 . 3.6751(8) ?
Fe K1 5 3.8177(13) ?
Fe K1 9_556 3.8177(13) ?
Ni O1 . 2.017(3) y
Ni O1 12_565 2.017(3) y
Ni O1 4_556 2.017(3) y
Ni O1 9_566 2.017(3) y
Ni O2 . 2.047(5) y
Ni O2 9_566 2.047(5) y
Ni K2 1_455 3.3685(10) ?
Ni K2 . 3.3685(10) ?
K1 O3 . 2.740(3) y
K1 O3 3 2.740(3) y
K1 O3 12 2.740(3) y
K1 O3 10_556 2.740(3) y
K1 O4 5_444 2.745(5) y
K1 O4 7_455 2.745(5) y
K1 O2 14_546 2.759(5) y
K1 O2 5_544 2.759(5) y
K1 As2 5_544 3.314(2) ?
K1 As2 5_444 3.423(2) ?
K1 K2 5_444 3.4357(8) ?
K1 K2 6_554 3.4357(8) ?
K2 O1 9_666 2.461(3) y
K2 O1 12_565 2.461(3) y
K2 O1 4_656 2.461(3) y
K2 O1 . 2.461(3) y
K2 O3 14_556 2.939(4) y
K2 O3 6_554 2.939(4) y
K2 O3 15 2.939(4) y
K2 O3 7 2.939(4) y
K2 As1 9_666 3.3193(7) ?
K2 As1 15 3.3193(7) ?
K2 As1 7 3.3193(7) ?
K2 As1 . 3.3193(7) ?
As1 O3 6_554 1.672(3) y
As1 O3 . 1.672(3) y
As1 O1 6_554 1.740(3) y
As1 O1 . 1.740(3) y
As1 K2 6_554 3.3193(7) ?
As1 K1 13 3.8049(9) ?
As2 O2 10_557 1.682(4) y
As2 O2 . 1.682(4) y
As2 O4 . 1.706(4) y
As2 O4 3_566 1.706(4) y
As2 K1 5_455 3.314(2) ?
As2 K1 5 3.423(2) ?
O2 K1 5_455 2.759(5) ?
O3 Fe 7_455 2.069(3) ?
O3 K2 6_554 2.939(4) ?
O4 Fe 13_556 2.051(3) ?
O4 K1 5 2.745(5) ?

_cod_database_fobs_code 2242050
